Charles Paillard,1, 2 _{Engin Torun,}3 _{Ludger Wirtz,}3 _{Jorge ´I˜}_{niguez,}4, 3 _{and Laurent Bellaiche}1

1_{Department of Physics and Institute for Nanoscience and Engineering,}

University of Arkansas, Fayetteville, Arkansas 72701, USA

2

Laboratoire Structures, Propri´et´es et Mod´elisation des Solides, CentraleSup´elec,

UMR CNRS 8580, Universit´e Paris-Saclay, 91190 Gif-sur-Yvette, France∗

3

Physics and Materials Science Research Unit, University of Luxembourg, 162a avenue de la Fa¨ıencerie, L-1511 Luxembourg, Luxembourg

4_{Materials Research and Technology Department,}

Luxembourg Institute of Science and Technology (LIST), Avenue des Hauts-Fourneaux 5, L-4362 Esch/Alzette, Luxembourg

Pattern notation Space Group

000/000 P m¯3m

000/00w+ _{P 4mm}

000/0+_{v}+_{v}+ _{Amm2}

000/u+u+u+ R3m

TABLE I. Correspondence between pattern notation used in the main manuscript and space group for BTO.

BRILLOUIN ZONE

The notation of the high symmetry point in the Bril-louin zone of the cubic P m¯3m phase is taken as follows: Γ = (0, 0, 0), X = (1/2, 0, 0), M = (1/2, 1/2, 0) and R = (1/2, 1/2, 1/2).

ATOMIC DISPLACEMENTS BTO

BTO is a classical ferroelectric which exhibits a tran-sition from a centrosymmetric cubic P m¯3m phase to a ferroelectric tetragonal P 4mm below ∼393 K with po-larization along the tetragonal axis [001], then to an orthorhombic structure Amm2 with polarization along a < 101 > pseudocubic direction below ∼280-270 K and finally to a rhombohedral R3m phase with polar-ization along a < 111 > pseudocubic direction below ∼183 K [1, 2].

In the main manuscript, we refer to those phases with respect to their dipolar and oxygen octahedra tilt pat-tern. The correspondence between the space group and pattern notation can be found in Table I

Moreover, the polar phase P 4mm atomic positions are [2]

• Ba (0, 0, 0)

• Ti (1/2, 1/2, 1/2 + δT i)

• Equatorial oxygens O, (1/2, 0, 1/2 + δO1) and (0, 1/2, 1/2 + δO1)

• Apical oxygen O, (1/2, 1/2, δO3)

In the Amm2 orthorhombic phase, the atoms have the following positions in pseudocubic axes:

• Ba (0, 0, 0)

• Ti (1/2 + δT i, 1/2− δT i, 1/2)

• Oxygens O, (δO1,1, 1/2− δO1,2, 1/2) and (1/2 + δO1,2,−δO1,1, 1/2).

• Apical oxygen O, (1/2 + δO3, 1/2− δO3, 0)

The rhombohedral R3m phase is characterized by the displacement pattern:

• Ba (0, 0, 0)

• Ti (1/2 + δT i, 1/2 + δT i, 1/2 + δT i)

• Oxygens O, (δO3, 1/2 + δO1, 1/2 + δO1), (1/2 + δO1, δO3, 1/2 + δO1), and (1/2 + δO1, 1/2 + δO1, δO3) The displacement pattern for those three phases is plotted in Fig. (1) as a function of the nph photocarrier

density, and shows the disappearance of any polar dis-placement in all three phases at around nph = 0.1 e/f.u.

The resulting phase is the cubic paraelectric P m¯3m state.

PTO

In Table II, we give the correspondence between the different pattern notations employed and the space group considered in the case of PTO.

In Fig. (2), we plot the displacement of atoms in PTO. The upper panel of Fig. (2) shows the displacement of the Ti, equatorial O1atoms and apical O3atom of the

0.00 0.05 0.10 0.15
nph (e/f.u.)
−0.1
0.0
displacemen
t
(˚A)
δT i
δO1
δO3
0.00 0.05 0.10 0.15
nph (e/f.u.)
−0.05
0.00
0.05
displacemen
t
(˚A) δ_{δ}T i
O,1
δO,2
0.00 0.05 0.10 0.15
nph (e/f.u.)
−0.05
0.00
0.05
displacemen
t
(˚A) δ_{δ}T i
O3
δO1,1
δO1,2

FIG. 1. Displacement pattern (top panel) for the P 4mm

phase, (middle panel) the R3m phase and (lower panel) the

Amm2 phase in BaTiO3.

Pattern notation Space Group

000/000 P m¯3m 000/0+0+w+ P 4mm − − −/u+ u+u+ R3c − − −/000 R¯3c 00 − /000 I4/mcm − − 0/u− ¯ u−0− Imma

TABLE II. Correspondence between pattern notation used in the main manuscript and space group for PTO.

of Fig. (2), the antiferroelectric (AFE) displacements in the Imma phase of Pb [ that are, (δP b,−δP b, 0)] atoms

and the O3 atom (1/2 + δO3, 1/2− δO3, 0), with mod-ulation vector R = (1/2, 1/2, 1/2) in pseudocubic axes, are depicted and show increase of the AFE order with nph. Concurrently, we have plotted the tilt angle of the

a−_{a}−_{c}0 _{Imma phase and a}−_{a}−_{a}−_{-tilted R3c and R¯}_{3c}

0.00 0.05 0.10 0.15
nph (e/f.u.)
−0.4
−0.3
−0.2
[001]
displacemen
t
δT i
δO1
δO3
0.05 0.10 0.15
nph (e/f.u.)
−0.3
−0.2
−0.1
0.0
[111]
displacemen
t
(˚A) _{δ}_{T i}
δO
0.00 0.05 0.10 0.15
nph (e/f.u.)
−0.2
−0.1
0.0
[1
¯ 10]
AFE
R
displacemen
t
(˚A)
δP b
δO3

FIG. 2. Displacement pattern (top panel) for the P 4mm

phase, (middle panel) the R3c phase and (lower panel) the

Imma phase in PbTiO3.

phases in PbTiO3 in Fig. (3). It is clear that the tilt

angle increases with nph consistent with the increased

instability at the R point in the phonon band structure of the paraelectric cubic phase presented in the main manuscript.

MINIMUM ENERGY PATH

correspond-0.00 0.05 0.10 0.15 ne(electron/u.c.) 1 2 3 4 5 ωR ( ◦ ) ωx,Imma ωy,Imma ωx,R¯3c ωy,R¯3c ωz,R¯3c ωx,R3c ωy,R3c ωz,R3c

FIG. 3. Tilt angle of the oxygen octahedron in the Imma,

R3c and R¯3c phases in PbTiO3.

0.0 0.2 0.4 0.6 0.8 1.0 λM EP 0 20 40 E − EP 4 mm (meV/f.u.) nph= 0.00e nph= 0.05e nph= 0.10e nph= 0.15e

FIG. 4. Energy change along the minimum energy path

(denoted by the adimensional parameter λM EP) linking the

P 4mm and Imma phases in PTO, for nph = 0.00 e/f.u.

(navy circles), nph = 0.05 e/f.u. (dodgerblue squares),

nph = 0.10 e/f.u. (yellow triangles) and nph = 0.15 e/f.u.

(red diamonds).

ing to nph = 0.10 e/f.u., in Figure 4) , hence creating

a metastable state in PTO. At larger concentration of photoexcited carriers (red diamonds in Figure 4), Imma even becomes stable compared to the P 4mm state!

ABOUT A MONOCLINIC PHASE IN BTO Let us discuss the presence of a monoclinic phase, in particular in BTO, that was reported experimentally both under illumination in nanowires [4] and through electron doping [5]. We attempted to construct a

0.00 0.05 0.10 0.15 nph (e/f.u.) 0 5 10 15 E − ER 3 m (meV/f.u.) Amm2 P m¯3m Cm P 4mm

FIG. 5. Energy of different phases in BTO with respect to

the 000/u+_{u}+_{u}+_{(R3m) structure (dashed dark line), which is}

the ground state in the dark, including that of the attempted Cm structure.

monoclinic Cm phase, however the relaxed structure
is structurally and energetically extremely close to the
000/u+_{u}+_{u}+_{and 000/00w}+_{phase. We thus cannot }

con-clude with certainty about the existence of a monoclinic phase as a ground state. Nonetheless, Fig. (5) shows the existence of multiple phases with different orienta-tions of the polarization in a close energy window near nph = 0.03 e/f.u., indicating flattening of the energy

landscape. We thus expect the appearance of a low sym-metry phase to bridge the rhombohedral and tetrago-nal phases, and large electromechanical properties, as is commonly found at morphotropic phase boundaries in relaxor-ferroelectric solid solutions [6, 7].

PARALLEL WITH HYDROSTATIC PRESSURE It is clear from Fig. (6) that most non-trivial phases (i.e., other than the cubic paraelectric phase 000/000) show a decrease in volume when carriers are photogen-erated. This is consistent with a reduction of the polar order and is also typically expected when a perovskite is subject to hydrostatic pressure. It is also interesting to note that Ref. [8] drew parallels between doping and hydrostatic pressure, and that Ref. [9] proposed that the potential-deformation mechanism could generate an ef-fective photo-induced stress.

However, we note that

• The volume of the cubic phase of BTO increases (see Fig. (6.a)) with nph; the volume of the cubic

phase in PTO is non-monotonous, starting to de-crease at low nph and then increasing at large nph

(see Fig. (6.b)).

un-note that the most stable phases at large
concentra-tions of photo-excited carriers are − − 0/u−_{u}_{¯}−_{0}−

or−−−/000. In other words, while the −−−/000
phase was previously reported above 20 GPa [12],
we predict here that_{− − 0/u}−_{u}_{¯}−_{0}−_{is more stable.}

In addition, 00_{− /00w}+ _{and}

− − 0/u−_{u}_{¯}−_{0}− _{}

pre-dicted or observed in Refs. [10, 11] are not stable phases here.

It is thus doubtful that the effect presently observed can be solely described in terms of hydrostatic pressure. Nonetheless, we not that Ref. [9] identified two sources of photo-induced deformations: (i) photo-induced stress, mediated by the potential-deformation mechanism (in other words roughly∝∂Eg

∂η , with η being the strain and

Eg the bandgap) and (ii) a combined action of the

con-verse piezoelectric effect and an effective photo-induced
electric field (_{∝} ∂Eg

∂P ). It would thus be interesting to

investigate whether the photo-induced transitions dis-cussed here can be understood as a suitable combination of applied external stresses and electric fields.

INTERATOMIC FORCE CONSTANTS
In Figure 7, we calculate the interatomic force
con-stants (IFCs) in 2_{× 2 × 2 supercells of the cubic phase in}
both BTO and PTO, for different concentration of
pho-toexcited carriers, using the PHONOPY package (version
1.14.2) [13]. The IFC are defined as

IF Cij,αβ = ∂Fi,α ∂τj,β = EKS ∂τi,α∂τj,β , (1)

and characterize the force felt by an atom i in direction α (α = X, Y or Z) when atom j is moved by an incre-ment δτj,β in direction β. In the cubic phase, IF CXX =

IF CY Y = IF CZZ and IF CY Z = IF CZX = IF CXY.

We plot IF CXX and IF CXY for different atom pairs

(e.g. Ti-O (first neighbors, located around 2 ˚A), etc.),
which we classify by distance separating the atom pairs i
and j in the supercell. It is clear in Figure 7 that for most
atom pairs, the IFCs are reduced under photoexcitation,
most notably the 4th _{neighbors (located around 4 ˚}_{A),}

and corresponding to Ti-Ti and O-O interactions. We also note that the reduction of the ”long range” forces, already discussed in Ref. [8], is consistent with the desta-bilization of the polar phase; indeed, polar order is mainly thought to originate from long range Coulomb interac-tion. Note however that, in doped (hence metallic) cases, short range ”metascreening” forces may represent a com-peting force towards the stabilization of some sort of po-lar order [8]. In our case, BTO is predicted to show a cubic non-polar character under large photoexcitation,

trons) [8]; in contrast, in PTO, although the ferroelectric instability survives in the phonon dispersion curves (most likely due to metascreening, according the calculation in Ref. [8]), it is overcome by the tilt instability (see Fig-ures 2e-h in the main manuscript).

MANY BODY CORRECTIONS TO THE BAND GAP

Density functional theory fails to accurately describe quasi-particle excitations. In particular, it is well known that the bandgap is, in general, underestimated. There-fore, we have performed G0W0 [19] calculations within

the plasmon-pole approximation to calculate the change in the bandgap and other modifications of the bandstruc-ture. We have used the Quantum Espresso [14, 15] code for the calculation of Kohn-Sham wave functions and en-ergies on the LDA level and then the Yambo [16, 17] pack-age for the G0W0corrections on the three relevant phases

in BaTiO3 and PbTiO3. We have used an 8× 8 × 8

k-point grid in the case of the cubic phase with 5 atom per unit cell (and corresponding k-meshes on the other phases that contain more atoms in the unit cell). A 30 Ry plane wave cut-off is chosen for the exchange self-energy computation; 60 and 260 bands are selected in the com-putation of the independent particle polarizability χ0and

the screening operator W , respectively.

In Tables III & IV, we present the bandgap as deter-mined in LDA and from G0W0for the three relevant BTO

and PTO phases. We note that the use of many-body
techniques mostly shifts rigidly the conduction band up,
as for example shown in the case of PTO 000/00w+ _{in}

Fig. 8. The bandgap correction is slightly different for the different phases, but the maximum variation is 90 meV for BTO and 140 meV for PTO. The correction is small-est for the non-polar phase, which further strengthens the result that non-polar phases are favored under illumina-tion. Although the concentration of electrons needed to actually perform the photo-induced transition will be al-tered, we conclude that it will not alter the realization of such transition. If anything, at least in BTO, it should actually lower the number of photoexcited carriers nec-essary to reach the transition. In addition, our phonon dispersion calculations (Fig. 2 of the main text) do reveal that the cubic phase tends to be stabilized in BaTiO3,

while in PbTiO3 antiferrodistortive phases tend to be

stabilized.

*0.000 0.025 0.050 0.075 0.100 0.125 0.150*
*nph* (e/f.u.)
*59.0*
*59.5*
*60.0*
*60.5*
*V*
(˚A
3 /f.u.)
*000/000*
*000/00w*+
*− − −/000*
*− − −/u*+* _{u}*+

*+*

_{u}*− − 0/u−*

_{¯}

_{u}−_{0}

*−*00

*− /000*

*0.000 0.025 0.050 0.075 0.100 0.125 0.150*

*nph*(e/f.u.)

*63.2*

*63.4*

*63.6*

*63.8*

*64.0*

*V*(˚A 3 /f.u.)

*000/000*

*000/00w*+

*000/u*+

*+*

_{u}*+*

_{u}*000/0*+

*+*

_{v}*+*

_{v}## (a)

## (b)

FIG. 6. Volume change of the 5-atom perovskite cell with concentration of photo-excited carriers nphin (a) BTO and (b) PTO.

## (a)

## (b)

## (c)

## (d)

## BTO

## PTO

FIG. 7. Interatomic Force Constants (IFCs) in the cubic phase for XX and XY components for BTO (a & b) and PTO (c &

d) for photoexcited carrier concentrations nph = 0.00 (blue circles), 0.05 (green square), 0.10 (gold diamond) and 0.15 e/f.u.

000/000 1.813/1.893 1.781/1.904 3.362/3.477 +1.549/+1.584

000/00w+ 1.833/2.109 1.817/2.225 3.437/3.725 +1.604/+1.616

000/u+u+u+ 2.130/2.359 2.286/2.634 3.769/4.014 +1.639/+1.655

TABLE III. Indirect and direct bandgap in BaTiO3 using the LDA approximation for the exchange-correlation energy, and

G0W0 corrections to take into account the many-body effects. The difference of bandgaps between the G0W0 and LDA

approximations are shown in the last column.

Phase Eindirectg,LDA /E

direct g,LDA (eV) E indirect g,G0W0/E direct g,G0W0 (eV) δE indirect g /δE direct g (eV) 000/000 1.539/1.550 3.000/3.007 +1.461/+1.457 000/00w+ 1.589/1.888 3.192/3.527 +1.603/+1.639

TABLE IV. Indirect and direct bandgap in PbTiO3 using the LDA approximation for the exchange-correlation energy, and

G0W0 corrections to take into account the many-body effects. The difference of bandgaps between the G0W0 and LDA

approximations are shown in the last column.

Γ X M Γ Z R A Z X R M A −4 −2 0 2 4 6 ε − εF (eV)

FIG. 8. LDA (black) and G0W0 (light blue) corrected band

structure of 000/00w+_{PTO.}

the level of the random-phase approximation for an ex-cited carrier occupation. Both are currently out of reach. However, the use of hybrid functionals within DFT allows to take approximately those effects into account. Calcu-lations are presented in the following section.

Furthermore, it is worth noting that, from time-resolved pump-probe experiments, the exciton lifetime is in general considered to be close to the picosecond because of inelastic scattering by phonons [18]. This is rather large compared to the radiative recombination life-time which is considered larger than a nanosecond [18]. As a result, one expects in a stationary regime that a large amount of photoexcited carriers are free band car-riers and follow a quasi-Fermi-Dirac distribution; only a small fraction of the photoexcited carriers will be

non-thermalized.

CALCULATIONS OF THE SOFT MODE STABILIZATION WITH HYBRID

FUNCTIONALS

**0.00**

**0.05**

**0.10**

**0.15**

**0.20**

**0.25**

**0.30**

**Charge**

**5**

**0**

**5**

**10**

**15**

**Frequency(THZ)**

**PBESOL**

**HSESOL**

**BTO**

FIG. 9. Phonon frequencies of the cubic phase of BTO

as a function of excited charge density (in electron/formula unit). We compare calculations performed with the semi-local PBEsol functional (black lines) and with the hybrid HSEsol functional (red lines).

mode is strongly influenced. At low excited charge den-sity it has negative (or, more precisely, imaginary) fre-quency. At an excited charge density of 0.09 – 0.1 elec-tron per formula unit, it is stabilized and converges to-wards an optical frequency at high charging. This be-haviour is qualitatively and semi-quantitatively the same for both functionals and it is consistent with the phonon dispersion in Fig. 2 of the main manuscript. The calcula-tions thus demonstrate that the stabilization mechanism is robust under changes in the band gap (as mimicked by different functionals) and under changes in the details of the excited states occupation (e.g., Fermi-Dirac distri-bution versus distridistri-bution with separate quasi-Fermi lev-els). Note that for the HSEsol functional the crossover is at slightly larger excited charge density than for the PBEsol functional. This may be considered to be in con-trast to our remark that the GW corrections seem to favor the stability of the cubic phase. Note, however, that the HSEsol functional (and its corresponding lattice optimization) leads to an increase of the lattice instabil-ity (reflected in the larger absolute value of the imaginary frequency) and thus needs a larger excited charge density in order to overcome this instability.

In addition, in Figs. 10a-b, we compare the band struc-tures obtained for cubic BTO with the PBESol and the HSESol exchange-correlation functionals. Apart from a rigid upshift of the conduction bands of the HSESol band structure, the band dispersions are similar across the two functionals. Furthermore, we further report the

### ampli-(a)

### (b)

Γ X M Γ R -3 -2 -1 0 1 2 3 4 5 E-Ef (eV) Γ X M Γ R -3 -2 -1 0 1 2 3 4 5 E-Ef (eV)### (c)

### (d)

### (e)

### (f)

FIG. 10. Band structures of cubic 000/000 BTO calculated using the (a) PBESol and (b) HSESol functionals with the CRYSTAL code. The isosurfaces of the wavefunctions cor-responding to the top of the valence band (c & e) and the bottom of the conduction band (d & f) are depicted for the PBESol and HSESol functionals respectively.

tude of the states at the top of the valence band in Fig. 10c and bottom of the conduction band in Fig. 10d for the PBESol functional in cubic BTO. Similar data are given in Figs. 10e and 10f but for the HSESol functional. No change in the atomic character of those states can be observed between those two functionals.

INFLUENCE OF THE

EXCHANGE-CORRELATION FUNCTIONAL We also tested the influence of the functional on the phonon dispersions and the total energy in the special case of BaTiO3. The main manuscript uses the PBESol

functional as it gives an overall rhombohedral ground
state structure which is closer to experiments than LDA.
Indeed, our lattice constants in the rhombohedral phase
of BTO in the electronic ground state are 3.963 ˚A and
89.927◦ _{in LDA, 4.002 ˚}_{A and 89.868}◦ _{in PBESol, while}

low temperature structural characterization experiments
show lattice constants of 4.004 ˚A and 89.839◦_{in Ref. [2].}

However, LDA calculations show qualitative agreement with the results obtained using the PBESol functional, as shown in Figs. 11 & 12.

∗

charles.paillard@centralesupelec.fr

[1] H. D. Megaw, Acta Crystallographica 5, 739 (1952). [2] G. H. Kwei, A. C. Lawson, S. J. L. Billinge, S. W.

Cheong, The Journal of Physical Chemistry 97, 2368 (1993).

[3] E. Weinan, W. Ren, E. Vanden-Eijnden, J. Chem. Phys. 126, 164103 (2007).

Γ X R M Γ R X M Γ 0 10 ¯hω (THz) Γ X R M Γ R X M Γ 0 10 ¯hω (THz) Γ X R M Γ R X M Γ 0 10 ¯hω (THz) Γ X R M Γ R X M Γ 0 10 ¯hω (THz)

FIG. 11. Phonon spectra of the cubic paraelectric high-symmetry phase of BTO using the LDA exchange-correlation functional,

for different excited carrier concentrations: from left to right, nph= 0, 0.05, 0.10 and 0.15 e/f.u.

0.00 0.05 0.10 0.15
nph (e/f.u.)
0
2
4
6
E
−
E000
/u
+u
+
u
+
(meV/f.u.)
000/0+_{v}+_{v}+
000/000
000/00w+

FIG. 12. Kohn-Sham energy of various phases in BTO using the LDA functional.

[6] Z.-G. Ye, B. Noheda, M. Dong, D. E¿ Cox, G. Shirane, Physical Review B 64, 184114 (2001).

[7] L. Bellaiche, A. Garc´ıa, D. Vanderbilt, Physical Review Letters 84, 5427 (2000).

[8] H. J. Zhao et al. Physical Review B 97, 054107 (2018). [9] C. Paillard, S. Prosandeev, L. Bellaiche, Physical Review

B 96, 045205 (2017).

[10] I. A. Kornev, et al. Physical Review Letters 95, 196804 (2005).

[11] P.-E. Janolin, et al. Physical Review Letters 101, 237601 (2008).

[12] M. Ahart, et al. Nature 451, 545 (2008).

[13] A. Togo, I. Tanaka, Scripta Materialia 108, 1 (2015). [14] P. Giannozzi, et al. J. Phys. Condens. Matter 21, 395502

(2009).

[15] P. Giannozzi, et al. J. Phys. Condens. Matter 29, 465901 (2017).

[16] A. Marini, C. Hogan, M. Gr¨uning, D. Varsano Comput.

Phys. Commun. 180, 1392–1403 (2009).

[17] D. Sangalli, A. Ferretti, H. Miranda, C. Attaccalite, I. Marri, E. Cannuccia, P. Melo, M. Marsili, F. Paleari,

A. Marrazzo, G. Prandini, P. Bonf`a, M.O. Atambo, F.

Affinito, M. Palummo, A. Molina-S´anchez, C. Hogan, M.

Gr¨uning, D. Varsano, A. Marini, arXiv:1902.03837

[cond-mat.mtrl-sci] (2019).

[18] C. Thomsen, H.T. Grahn, H.J. Maris, and J. Tauc, Phys. Rev. B 34, 4129 (1986).

[19] M. S. Hybertsen, S. G. Louie, Phys. Rev. B 34, 5390 (1986).

[20] L. Schimka, J. Harl, and G. Kresse, J. Chem. Phys. 134, 024116 (2011).

[21] R. Dovesi, A. Erba, R. Orlando, C. M. Zicovich-Wilson, B. Civalleri, L. Maschio, M. Rerat, S. Casassa, J. Baima, S. Salustro, B. Kirtman, WIREs Comput Mol Sci. 8, e1360 (2018)